{'fraction_non_alphanumeric': 0.019700551615445233, 'fraction_numerical': 0.007880220646178092, 'mean_word_length': 5.018957345971564, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Comparison of SiGe Virtual Substrates for the Fabrication of Strained Silicon-on-Insulator (sSOI) Using Wafer Bonding and Layer Transfer

Different methods of preparing sSOI wafers have been analyzed. The initial virtual substrate wafers are characterized by a 17 20 nm thick strained silicon layer grown either on a thick relaxed SiGe layer on a graded buffer or on a thin SiGe buffer relaxed by He implantation. Bonding and layer transfer experiments using different oxide layers proved that strained silicon layers are completely transferred if designed PE-CVD oxide layers were used. For both types of virtual substrates the oxide layers are deposited on top of the strained silicon and bonded to non-oxidized (blank) silicon wafers. A perfect layers transfer is obtained for virtual substrates having thick SiGe buffer layers (type A) even at 350°C, while annealing at 450 °C is required for substrates with thin SiGe buffer layers (type B). The lower annealing temperature for substrates of type A is caused by the lower activation energy for blistering. The hydrogen implantation is here into the SiGe. For type B substrates the hydrogen implantation is into the underlying Si requiring a higher temperature for layer splitting (higher activation energy for Si).